Attribution-NonCommercial-NoDerivatives 4.0 International (CC BY-NC-ND 4.0) license http://dx.doi.org/10.22201/fi.25940732e.2019.20n4.040
El propósito de este trabajo es evaluar la protección contra la corrosión y el desgaste de un sustrato de acero mediante recubrimien-tos nanocompuesrecubrimien-tos de epoxi-vinil éster y nanopartículas de Zn y TiO2. Los sustratos de acero se recubrieron con nanocompuestos de epoxi-vinil éster, variando las concentraciones de nanopartículas de Zn y TiO2 y las combinaciones de ambas nanopartículas. La resistencia a la corrosión se evaluó mediante la prueba de niebla salina durante 480 h, según la norma ASTM B-117. El grado de daño se obtuvo cuantitativamente al medir la mejora en el área corroída en comparación con la marca trazada en los especímenes. La evaluación tribológica se realizó con una configuración de bola-sobre-disco, de acuerdo con la norma ASTM G-99. Los resultados mostraron que la combinación de nanopartículas de Zn y TiO2 en un recubrimiento epoxi-vinil éster proporciona un efecto sinérgico, mejorando la protección contra la corrosión debido a sus mecanismos combinados de corrosión y reducción tribológica.
Descriptores: Nanocompuestos, corrosión, resistencia al desgaste, nanopartículas, resina epóxica.
The purpose of this paper is to evaluate the corrosion and wear protection of a steel substrate by epoxy vinyl ester nanocomposite coatings with Zn and TiO2 nanoparticle fillers. Steel substrates were coated with epoxy vinyl ester nanocomposites, varying Zn and TiO2 nanofiller concentrations and combinations of both nanoparticles. Corrosion resistance was evaluated by salt spray fog test du-ring 480 h, according to ASTM B-117. The degree of damage was obtained quantitatively by measudu-ring the enhancement in corro-ded area compared to the scribe mark. Tribological evaluation was performed with a ball-on-disk tribotester, according to ASTM G-99. Results showed that the combination of Zn and TiO2 nanofillers in an epoxy vinyl ester coating provide a synergistic effect, enhancing corrosion protection due to their combined corrosion and tribological reducing mechanisms.
Synergistic effect of nanocoatings for corrosion and wear protection of steel surfaces
Efecto sinérgico de nanorecubrimientos para la protección contra la corrosión y el
desgaste de superficies de acero
Taha-Tijerina Jaime Universidad de Monterrey Departamento de Ingeniería E-mail: email@example.com http://orcid.org/0000-0001-6781-9414 Peña-Parás Laura
Universidad de Monterrey Departamento de Ingeniería E-mail: firstname.lastname@example.org https://orcid.org/0000-0002-7580-6995 Sánchez-Fernández Antonio
Instituto Tecnológico de Estudios Superiores de Monterrey Departamento de Química
Maldonado-Cortés Demófilo Universidad de Monterrey Departamento de Ingeniería
Corrosion is an aggressive effect over material perfor -mance and degradation under working environments, which is a natural inevitable process. Corrosion is a se -vere problem that affects several industry fields, such as infrastructure, transportation, utilities, production and manufacturing, as it causes premature failure of metallic components (Koch, 2002); typically for ferrous metals, manifesting as unsightly red rust or paint/coa -ting blistering. The estimated worldwide losses due co -rrosion exceed $1.8 trillion, annually (Schmitt et al., 2009).
One of the most common means to reduce corrosion is through the application of organic coatings (Akinci & Yilmaz, 2011; Bierwagen, 1998). Coatings are generally exposed to different environments and working condi -tions, hence they may require a set of properties such as adhesion, high hardness, high toughness, high corro -sion and oxidation resistance, among others. Recently, nanoparticles have been incorporated into matrices in order to improve corrosion protection, barrier proper -ties, filling pores and voids in the matrix, and increase overall mechanical properties, including wear resistan -ce (Abdullayev et al., 2013; Barna et al., 2005; Guin et al., 2015; Gusev et al., 1998; Lam & Lau, 2006; Li et al., 2013; Sababi et al., 2014; Wang & Zhang, 2010).
Regarding corrosion performance, Hamdy and Butt (2007) were able to successfully evaluate the effect of chromate conversion coatings for the corrosion protec -tion of aluminum alloys. It was observed that vanadia treatments improve the corrosion resistance due to the formation of highly protective vanadium oxides, as Va -nadium combines through the pores of Al-oxide layer to form thick Al–V-oxide layer. Due to the buffering ac -tion of vanadium, it plays an important role to reject the chloride ions from the material surface. Feng et al. (Wang et al., 2010c) proposed nano-Al2O3 particles in -corporation to composite coatings in order to improve the corrosion and oxidation resistance. Moreover, Mon -temor (2014) reviewed the most recent self-healing and smart coating alternatives for enhanced corrosion pro -tection. Poor adhesion between substrate and coating may cause spalling and delamination of the coating, which can be largely controlled by relieving residual stresses from the coatings (Harish et al., 2010). For ins -tance, epoxy coatings containing 1.0 wt. % of Zn, SiO2, Fe2O3, and halloysite clay nanoparticles have been applied to steel substrates, reducing the corrosion rate by 11 to 910 times after immersion in a 3 % NaCl solu -tion for over 28 days (Shi et al., 2009). Alkyl-based waterborne coatings filled with ZnO improved abra
-sion and scratch resistance, and showed little changes on the surface topography after salt-spray evaluations (Dhoke et al., 2009). Furthermore, a study varying the nano-TiO2 particle size (10-150 nm) demonstrated that smaller nanoparticles increase corrosion inhibition effi -ciency and lower permeability to corrosion agents (De -yab & Keera, 2014). Similarly, other investigations have combined diverse particle additives achieving a syner -gistic effect (Lu et al., 2016).
Wear resistance of polymer coatings has also been improved with nanoparticle reinforcements, as has been observed by several authors (Bahadur et al., 1994; Cho & Bahadur, 2005; Jia et al., 2006; Wang et al., 2003; Wang et al., 2010b; Xian et al., 2006). It has been found that physical characteristics are not significantly affec -ted; due to the particles small size, nanoparticles do not affect the transparency or the gloss of coatings. Further -more, nanocoatings can thus be used to maintain the surface appearance and durability as well. Polymer coatings form transfer films of metal counterfaces upon friction, this effect is enhanced with nanoparticle addi -tives (Friedrich & Schlarb, 2011). For example, Barna et al. (2005) investigated the incorporation of diverse oxi -de-based nanostructures to improve hardness and me -chanical performance of coatings, thereby improving their wear and scratch resistance.
A synergistic effect has been observed when diffe -rent nanoparticles have been combined (Jia et al., 2006; Wang et al., 2010b; Xian et al., 2006). Wang et al. (2003) for instance, reported a synergistic action in the tribolo -gical behavior of polyamide composites made with car -bon fiber and micro-size MoS2 filler. The aim of our study is to develop a nanocomposite for corrosion and wear protection of steel substrates, with an epoxy vinyl ester coating and nanoparticles reinforcements; varying filler fractions and mixtures of Zn and TiO2 nanostruc -tures, and determine the presence of a synergistic co -rrosion and wear protection effect.
The epoxy vinyl ester resin Derakane Momentum 411-350, Cobalt Naphthenate (Cobalt 6 %), and Methylethylketone Peroxide (MEKP) NOROX MEKP-925H catalyst were obtained from Ashland. Nanoparti -cles of Zn ( < 50 nm, spherical) and TiO2 ( < 21 nm, spherical) were obtained from Sigma Aldrich. Scanning electron micrographs of these nanoparticles are shown in Figure 1.
Figure 1.Scanning electron micrographs of nanoparticles of: a) TiO2 and b) Zn
Steel substrates of an AISI 1045 steel measuring 150 mm by 100 mm with 2.0 mm in thickness were sanded and washed with acetone to remove any rust and dirt from the surface. Next, surfaces were sanded with 220-grit sandpaper to an Ra of 0.48 µm. Nanocomposite coatings at various concentrations and combinations of Zn and TiO2 nanoparticles within an epoxy vinyl ester resin were prepared as shown in Table 1. This resin is widely used for coatings and as a matrix for composite mate -rials. In order to break large agglomerates, nanoparti -cles were first dispersed in the neat resin using an Ultra Turraz T10 homogenizer for 5 min, followed by 2 min sonication with a Cole-Parmer 750-Watt ultrasonic ho -mogenizer at room temperature (25 °C). Then, 0.05 parts per hundred (phr) of Cobalt Napthenate 6 % and 1.00 phr of methyl ethyl ketone peroxide (MEKP) ca -talyst were added to the resin mixtures in order to har -den the composite. Curing time of resin was 30 ± 10 min at 35 °C. Lastly, polymer nanocoatings were uniformly applied with a brush and allowed to cure for 24 h. The thickness of coatings was 150 µm, measured by an Elco -meter 456 coating thickness gauge.
Coated samples were scribed per ASTM 1654, and pla -ced in an automatic salt chamber at a 60 ° angle using a Harshaw/Filtrol salt spray cabinet for 480 h. Five samples were prepared and teste for each nanocompo -site coating, according the Dixon statistical methodo -logy (Dean & Dixon, 1951; Rorabacher, 1991). Tests were run according to ASTM B-117. The tests were conducted at 35 °C with a spray of 5 % NaCl solution, pH of 6.5 - 7.2, and 96 % relative humidity. Samples were scanned and analyzed according to ASTM D-7087 and monitored after 96, 168, 288, 336, 408, and 480 h., respectively, measuring the increase in corro -ded area from the scribe mark.
Tribological properties of nanocomposite coatings were determined with a ball-on-disk tribotester (Figure 2a), under ASTM G-99, to determine the wear resistance with an accelerated test under point contact conditions. Here, the coatings are subjected to a load of 25 N, speed of 238 rpm, over a total distance of 100 m and wear track diameter of 16 mm (Figure 2b). With this method an increase in the friction force is observed when the coating layer breaks, and thus the duration of the coa -ting is obtained. Higher duration and wear resistance of coatings is beneficial for delaying corrosion initia -tion. Figure 2c shows the friction force through time; it could be seen that at 750 s, the coating layer is broken, and friction force increases.
Table 1.Preparation of epoxy vinyl ester polymer nanocomposite coatings
Sample number Nanoparticle
Zn (wt. %) TiO2 (wt. %)
1 Neat resin
-5 - 0.1
6 - 0.5
7 - 1.0
8 0.1 0.1
9 0.1 0.5
10 0.1 1.0
11 0.5 0.1
12 0.5 0.5
13 0.5 1.0
14 1.0 0.1
15 1.0 0.5
rEsults and dIscussIon
Figure3 shows the general appearance of scribed coa -ted steel surfaces prior to the salt spray test. Images of samples after exposure for 96 h, and 480 h are shown in Figure 4 and Figure 5, respectively.
Figure 3.Aspect of coated samples (100mm by 150mm - 4 by 6 in.) before salt spray test
As expected, the highest degree of corrosion is found for the neat resin specimen (sample 1). Corrosion products are found around the scribes for all samples; even at 96h, as shown in Figure 4. In general, in both images, Figure 4 and Figure 5, the least amount of rust is found on the surfaces of samples combining different proportions of mixtures of Zn and TiO2 nanoparticles, compared to samples with only one type of nanoparti -cle, this was observed qualitatively.
Figure 6 and Figure 7 depict the growth of the corro -ded area with respect to the scribed mark obtained through image analysis performed with 2D CAD sys
-tem, in accordance to ASTM D-7087. Images were taken and analyzed at 96, 168, 288, 336, 408, and 480 h, and compared to the neat resin coating. The epoxy vinyl ester resin presented a rapid increase in corroded area (150 %) after 96 h of exposure, after which the increase was lower. At 480 h the neat resin had an increase of 200 %, whereas all nanoparticle concentrations and mixtures showed better corrosion protection. In Figure 6 results showed an increasing corrosion protection rate up to 0.5 wt. %, after which a reverse trend was present, most likely due to filler agglomeration, particularly for TiO2, as has been observed from previous research and work in our group (Peña et al., 2014, 2015, 2016). In general, this nanoparticle showed better performance compared to Zn. For instance, at 0.1 and 0.5 wt.% TiO2 (Figure 6a) had a lower increase of corroded area at 480 h; 115 % and 44 %, respectively. This could be attributed to increased barrier properties against oxygen and water (Chen et al., 2006; Deyab & Keera, 2014) and due to filling the coa -tings’ pores and voids (Moazeni et al., 2013). The obser -ved increase at 1.0 wt. % TiO2 after 288 hrs under corrosion evaluation could be attributed to certain ten -dency of the nanoparticles to agglomerate, due to filler fraction, and form clusters, which diminished the protec -tion in the coating. Zn nanoparticles (Figure 6b) showed a rapid increase on corroded area after 96 h, similar to the neat resin, and an increase on area failed from scribe of ∼200 %, 107 %, and 116 % at 0.1, 0.5, and 1.0 wt. %, respectively at the end of the test.
found at a fixed 0.5 wt. % concentration of Zn (Figure 7b), where increase of ~ 26 % where found at 96 h expo -sure, and up to ~ 50 % increase was observed at 480 h, with increasing TiO2 filler fraction. Similar trends are observed at 1.0 wt. % Zn nanocomposite (Figure 7c); here the lowest corroded area was found with 0.5 wt. % TiO2, starting at 14 % and ending at 26 %. Thus, the best protection was observed for coatings with mixtures of 1.0 wt % Zn and 0.5 wt. % TiO2.
These results can be attributed to the combined effect of TiO2 and Zn enhancing barrier properties and lowering of different sizes of pores and voids volumes on polymer coatings. Therefore, this shows that the addition and combination of Zn and TiO2 resulted in a
synergistic effect, taking advantage of both nanoparti -cles’ corrosion reducing mechanisms.
Ball-on-disk tribotester was used for evaluations of tri -bological performance. Figure 8 depicts the synergis -tic effect of nanopar-ticle filler fraction and the coating duration under a constant load of 25 N. This result is determined when the coating breaks and the friction force increases, as shown in Figure 2c. Figure 8a shows that duration of the coating is improved with Zn and TiO2 nanoparticles with up to 0.5 wt. % up to 211 s, compared to 43 s for the unfilled polymer coating. Figure 4.Images of coated samples after exposure in salt spray for 96 h
When both nanoparticles are combined (Figure 8b) the duration increases up to 1000 s, with an improvement greater than 2000 %, compared to the pure epoxy vinyl ester polymer resin.
Figure 9 shows the depth wear rate in µm/s obtai -ned taking the displacement of the tribosystem that oc -curs in the z-axis (perpendicular to the disk surface) measured by the equipment and dividing it by the du -ration of the coating. For instance, in Figure 9a both Zn and TiO2 nanocomposites showed a decrease in depth wear rate compared to the neat resin with concentra -tions of 0.1 wt. % and 0.5 wt. %. The lowest wear rate, with a reduction of 89 %, is found for 0.5 wt.% Zn %. These enhancements can be explained as follows: it has been proposed that during the wear process nanoparti -cles could be slightly detached from the polymer ma
-trix and provide a rolling bearing effect, enhancing the protection to the polymer nanocomposite coating (Frie -drich & Schlarb, 2011). Furthermore, hardness of poly -mer nanocomposites increases with nanoparticle content, also lowering wear (Chen et al., 2006; Lingaraju
et al., 2011; Zhi et al., 2001). However, at higher concen -trations of Zn and TiO2 nanocomposites (1.0 wt. %) the wear rate increases, hence, the time for oxide to appear (layer duration). This may be due to nanoparticle agglo -meration in the matrix. In Figure 9b, where 0.1 wt. %, 0.5 wt. %, and 1.0 wt. % Zn nanocomposite coatings were prepared with varying concentrations of TiO2;it was observed that all combinations decreased depth wear rate demonstrating a synergistic effect between the selected nanoparticles with improvements up to 95 %. Consistent with Wang´s study (Wang et al., 2010b), it
Figure 6. a) Comparison of the area failed from scribe versus time for TiO2 nanocomposites, b) Zn nanocomposite coatings
is proposed that the small sized TiO2 aid in the filling of pores and voids of the matrix providing a load-bearing effect, whilst Zn nanoparticles provide a rolling-bea -ring effect, thus further reducing wear rate of polymer nanocomposites
Epoxy vinyl ester nanocomposite coatings were prepa -red with Zn and TiO2 nanofillers at various concentra -tions. The salt spray corrosion test showed that separately, both Zn and TiO2 improved the corrosion protection of steel substrates. However, when nanopar -ticles were combined, a synergistic effect was observed with lower percentage of corroded area, with the coa -ting of 1.0 wt. % Zn and 0.5 wt. % TiO2 having the best performance. This is attributed to smaller void volumes and enhanced barrier properties by adding TiO2 and Zn. Similar results were obtained by the tribological tests performed with a ball-on-disk tribometer. Indivi -dual nanoparticles provided an increase on wear resis -tance, but when both are combined the results are enhanced. In this case, the proposed tribological me -chanism is a load-bearing effect coupled with rolling-bearing mechanism by removal of nanoparticles during the wear process.
Authors want to thank the UdeM personnel, particu -larly José Nájera for their support on this work.
Abdullayev, E., Abbasov, V., Tursunbayeva, A., Portnov, V., Ibrahimov, H., Mukhtarova, G. & Lvov, Y. (2013). Self-healing
coatings based on halloysite clay polymer composites for pro
-tection of copper alloys. ACS Applied Materials Interfaces, 5
(10), 4464-4471. https://doi.org/10.1021/am400936m
Akinci, A. and Yilmaz, F. (2011). The effect of epoxy-polyester sea
-ling of sprayed metal coatings for additional corrosion protec
-tion. Anti-Corrosion Methods and Materials, 58 (1), 26-30. https://
Bahadur, S., Fu, Q. & Gong, D. (1994). The effect of reinforcement and the synergism between CuS and carbon fiber on the wear
of nylon. Wear, 178 (1), 123-130.
Barna, E., Bommer, B., Kürsteiner, J., Vital, A., Trzebiatowski, O., Koch, W., Schmid, B. & Graule, T. (2005). Innovative, scratch proof nanocomposites for clear coatings. Composites Part A. Applied Science and Manufacturing, 36 (4), 473-480.
Bierwagen, G.P. (1998). Corrosion and its control by coatings. In Organic coatings for corrosion control, Vol. 689, 1-8.
Chen, Y., Lin, A. & Gan, F. (2006). Improvement of polyacrylate coa
-ting by filling modified nano-TiO2. Applied Surface Science, 252
(24), 8635-8640. http://dx.doi.org/10.1016/j.apsusc.2005.11.083
Figure 8.a) Duration of polymer nanocomposite coatings with varying concentrations of Zn and TiO2 nanoparticles, compared to the neat resin, b) duration of polymer nanocomposite coatings of 0.1, 0.5, and 1.0 wt. % Zn with varying concentrations of TiO2 nanoparticles, compared to the neat resin
Cho, M.H. & Bahadur, S. (2005). Study of the tribological synergis
-tic effects in nano CuO-filled and fiber-reinforced polyphen
-ylene sulfide composites. Wear, 258 (5), 835-845. http://dx.doi.
Dean, R.B., & Dixon, W.J. (1951). Simplified statistics for small
numbers of observations. Analytical chemistry, 23 (4), 636-638.
Deyab, M.A. & Keera, S.T. (2014). Effect of nano-TiO2 particles
size on the corrosion resistance of alkyd coating. Materials
Chemistry and Physics, 146 (3), 406-411. https://doi.org/10.1016/j. matchemphys.2014.03.045
Dhoke, S.K., Khanna, A.S. & Sinha, T.J.M. (2009). Effect of nano-ZnO particles on the corrosion behavior of alkyd-based
waterborne coatings. Progress in Organic Coatings, 64 (4),
Friedrich, K. & Schlarb, A.K. (2011). Tribology of polymeric nanocom-posites: Friction and wear of bulk materials and coatings. Oxford: Elsevier Science.
Guin, A.K., Bhadu, M., Sinhababu, M., Rout, T.K. & Udayabhanu,
G. (2015). Effect of nano ZnO containing sol-gel coating on gal
-vanised iron sheet. Pigment Resin Technology, 44 (4), 239-249.
Gusev, A.I. (1998). Effects of the nanocrystalline state in solids. Physics-Uspekhi, 41 (1), 49-76.
Hamdy, A.S. & Butt, D.P. (2007). Novel anti-corrosion nano-sized
vanadia-based thin films prepared by sol-gel method for alu
-minum alloys. Journal of Materials Processing Technology, 181
(1), 76-80. http://dx.doi.org/10.1016/j.jmatprotec.2006.03.042
Harish C. Barshilia, Deepthi, B. & Rajam, K.S. (2010). Transition
metal nitride–based nanolayered multilayer coatings and na
-nocomposite coatings as novel superhard. In Nanostructured
Thin Films and Coatings. CRC Press, 427-480. http://dx.doi.
Huai-Qi, S., Qi-Bin, Z., Wen-Li, H., Bei-Bei, X., Zhong-Ping, X. &
Gui-Bai, H. (2011). A low temperature process for the applica
-tion of three-layer polyethylene coatings. Anti-Corrosion
Methods and Materials, 58 (6), 312-314.
Jia, Q.M., Zheng, M., Xu, C.Z. & Chen, H.X. (2006). The mechanical properties and tribological behavior of epoxy resin composites
modified by different shape nanofillers. Polymers for Advanced
Technologies, 17 (3), 168-173. https://doi.org/10.1002/pat.710
Koch, G.H., Brongers, M., Thompson, N.G., Virmani, Y.P. & Pa
-yer, J.H. (2002). Corrosion cost and preventive strategies in the
Lam, C.K. & Lau, K.T. (2006). Localized elastic modulus distribution
of nanoclay/epoxy composites by using nanoindentation.
Com-posite Structures, 75 (1-4), 553-558. http://dx.doi.org/10.1016/j. compstruct.2006.04.045
Li, X., Nikiforow, I., Pohl, K., Adams, J. & Johannsmann, D. (2013). Polyurethane coatings reinforced by halloysite nanotubes. Coatings, 3 (1), 16-25.
Lingaraju, D., Ramji, K., Pramila-Devi, M. & Rajya-Lakshmi, U. (2011).
Mechanical and tribological studies of polymer hybrid nanocom
-posites with nano reinforcements. Bulletin of Materials Science, 34
(4), 705-712. http://dx.doi.org/10.1007/s12034-011-0185-2
Lu, H., Yao, Y., Yin, J. & Lin, L. (2016). Functionally graded carbon nanotube and nafion/silica nanofibre for electrical actuation
of carbon fibre reinforced shape memory polymer. Pigment
Resin Technology, 45 (2), 93-98. https://doi.org/10.1108/PRT-05-2015-0048
Mathivanan, L. & Radhakrishna, S. (1998). Protection of steel structures in industries with epoxy-silicone based coatings. Anti-Corrosion Methods and Materials, 45 (5), 301-305.
Moazeni, N., Mohamad, Z., Faisal, N.L.I., Tehrani, M.A. & Dehbari, N. (2013). Anticorrosion epoxy coating enriched with hybrid
nanozinc dust and halloysite nanotubes. Journal of Applied
Poly-mer Science, 130 (2), 955-960. https://doi.org/10.1002/app.39239
Montemor, M.F. (2014). Functional and smart coatings for corro
-sion protection: A review of recent advances. Surface and
Coa-tings Technology, 258, 17-37.
Peña-Parás, L., Taha-Tijerina, J., García, A., Maldonado, D., Gon
-zález, J.A., Molina, D., Palacios, E. & Cantú, P. (2014). Anti
-wear and extreme pressure properties of nanofluids for
industrial applications. Tribology Transactions, 57 (6),
Peña-Parás, L., Taha-Tijerina, J., García, A., Maldonado, D., Nájera, A., Cantú, P. & Ortiz, D. (2015). Thermal transport and tribological
properties of nanogreases for metal-mechanic applications. Wear,
332-333, 1322-1326. https://doi.org/10.1016/j.wear.2015.01.062
Peña-Parás, L., Taha-Tijerina, J., Maldonado-Cortés, D., García-Pineda, P., Garza, G.T., Irigoyen, M., Gutiérrez, J. & Sánchez, D. (2016). Extreme pressure properties of nanolubricants for
metal-forming applications. Industrial Lubrication and
Tribolo-gy, 68 (1), 30-34. http://dx.doi.org/10.1108/ILT-05-2015-0069
Rorabacher, D.B. (1991). Statistical treatment for rejection of de
-viant values: critical values of Dixon’s “Q” parameter and re
-lated subrange ratios at the 95 % confidence level. Analytical
Chemistry, 63 (2), 139-146. https://doi.org/10.1021/ac00002a010 Sababi, M., Pan, J., Augustsson, P.-E., Sundell, P.-E. & Claesson, P.M. (2014). Influence of polyaniline and ceria nanoparticle additives
on corrosion protection of a UV-cure coating on carbon steel.
Co-rrosion Science, 84, 189-197. http://dx.doi.org/10.1016/j.cors -ci.2014.03.031
Schmitt, G.A., Schütze, M., Hays, G.F., Burns, W., Han, E., Pourbaix,
A. & Jacobson, G. (2009). Global needs for knowledge development
in materials deterioration and corrosion control in cooperation with. federal highway administration, FHWA-RD-01, 1-44.
Shi, X., Nguyen, T.A., Suo, Z., Liu, Y. & Avci, R. (2009). Effect of nano
-particles on the anticorrosion and mechanical properties of epo
-xy coating. Surface and Coatings Technology, 204 (3), 237-245. Wang, H. & Zhang, S. (2010). Toughness and toughening of hard
nanocomposite coatings. In Zhang S. (Ed.), Nanostructured thin films and coatings mechanical properties. CRC Press, 99-145. Wang, J., Gu, M., Songhao, B. & Ge, S. (2003). Investigation of the
-bon fiber reinforced nylon 1010 composites. Wear, 255 (1),
Wang, Q., Zhang, X. & Pei, X. (2010). Study on the synergistic effect of carbon fiber and graphite and nanoparticle on the friction
and wear behavior of polyimide composites. Materials Design,
31 (8), 3761-3768. http://dx.doi.org/10.1016/j.matdes.2010.03.017
Wang, Z., Han, E., Liu, F. & Ke, W. (2010). Fire and corrosion resis
-tances of intumescent nano-coating containing nano-SiO2 in
salt spray condition. Journal of Materials Science Technology, 26
(1), 75-81. https://doi.org/10.1016/S1005-0302(10)60012-6
Xian, G., Walter, R. & Haupert, F. (2006). A synergistic effect of nano-TiO2 and graphite on the tribological performance of
epoxy matrix composites. Journal of Applied Polymer Science,
102 (3), 2391-2400. https://doi.org/10.1002/app.24496
Zhi-Rong, M., Qiu-Zhang, M., Liu, H., Zeng, H., Wetzel, B. & Frie
-drich, K. (2001). Microstructure and tribological behavior of
polymeric nanocomposites. Industrial Lubrication and